Loading in 2 Seconds...
Loading in 2 Seconds...
Novel Approach to Achieve High ZT Thermoelectric Materials Helmut Baumgart 1,2 1 Department of Electrical and Computer Engineering Old Dominion University, Norfolk, Virginia 23529, USA 2 Applied Research Center at Thomas Jefferson National Accelerator Laboratories Newport News, Virginia 23606, USA 83rd Annual Meeting of the American Physical Society Southeastern Section Charlottesville, Virginia November 11 , 2016 Frank Batten College of Engineering & Technology Old Dominion University: www.eng.odu.edu
Outline • Introduction to Thermoelectric Principles • Methods to Enhance Thermoelectric Conversion Efficiency • Experiments • Thermoelectric nanolaminate Films of ALD Bi2Te3/Sb2Se3 • Case study ALD Synthesis of PbTe/ PbSe thermoelectric Nanolaminates • Use of Porous Templates & Nanostructuring to improve Figure of Merit • Seebeck Measurements of structured ALD thermoelectric Nanolaminates • Results and Discussions • Conclusions
Introduction TE cooler: Telecoms laser Waste Heat recovery to generate green energy Solar + Thermoelectrics constitute green renewable energy !! Microprocessor cooler NASA Voyager I & II Source:http://images.sciencedaily.com/2011/09/110920120238-large.jpg
Addressed Problem Thermoelectric energy conversion holds large promise in applications spanning from improved efficiency car engines to the energy sources of satellites,to converting industrial waste heat etc. However, the conversion efficiency of thermoelectric devices is sizably lower than practically needed. • Engineering Strategies to Improve the thermoelectric Figure of Merit • (1) ZT is maximized when the average electron energy deviates from the Fermi energy • (2) To optimize σ, increase the number of free carriers • (3) To minimize k, increase phonon scattering => decrease thermal conductivity • (4) to further decrease thermal conductivity utilize porous templates • (5) We propose Nanostructuring & Porous Templates for Phonon Engineering
Concept of Thermoelectric Generator • Strategy to improve Figure of Merit ZT • The efficiency of a thermoelectric material is determined by the dimensionless thermoelectric figure of merit, • ZT = σS2T/ κ • where S is the Seebeck coefficient, σ is the electrical conductivity, and κ is the thermal conductivity. The thermal conductivity actually is consisting from electron and phonon contributions • κ = κ e+ κ p • To improve upon the ZT, the Seebeck coefficient and electrical conductivity must increase, whereas the thermal conductivity κ must decrease. • The ZT of the material is related to the efficiency η of the Thermoelectric device, • where γ is the Carnot efficiency and Thotand Tcoldare temperatures (in K) of the hot and cold side of the TE material. Schematics of principle of thermoelectric generator
Phonon glass electron crystal Methods to Enhance TE Conversion Efficiency Glass-like thermal conductivity Crystal-like electronic properties • NanostructuredTE materials Phonon Scattering Mechanism and Electrons Transport within TE Materials Chen, Zhi-Gang, et al. Progress in Natural Science: Materials International 22.6 (2012): 535- 549. (a) bulk material, (b) 2-D structure, (c) 1-D structure, (d) 0-D structure • Phononic crystal (PnC) nanostructure Mid / long wavelength phonon Short wavelength phonon Hot electrons Cold electrons 2D Phononic Crystal, square lattice period =300 nm M. Nomura et al. Physical Review B 91, 205422 (2015). Phonon thermal conductivity for different configurations. G. Romano et al. Appl. Phys. Lett. 105, 033116 (2014).
Efficiency of Thermoelectric (TE) Material • The conversion efficiency of TE materials is related to a quantity, figure of merit ZT, which is defined as: Where S: Seebeck coefficient 𝜎: Electrical conductivity T：Temperature кe: Thermal conductivity due to electrons кL : Thermal conductivity due to phonons or lattice vibrations Illustration of the variation of the Seebeck coefficient S, electrical conductivity 𝜎 ,and thermal conductivity k as a function of the charge carrier concentration n for bulk material. C. Wood, Materials for thermoelectric energy conversion, Reports on Progress in Physics 51(1988)
State-of-the-art Figures of Merit ZT for Various Classes TE Materials Source: Thermoelectrics handbook :Macro to nano Edited by D.M.Rowe • Different TE materials work only for specific temperature application range. Major milestones achieved for ZT as a function of both year and temperature Vineis, Christopher J., et al. "Nanostructured thermoelectrics: big efficiency gains from small features." Advanced Materials 22.36 (2010): 3970-3980.
Phonon glass electron crystal • Methods to Enhance TE Conversion Efficiency Glass-like thermal conductivity Crystal-like electronic properties Generation of dislocation arrays during the liquid-phase compaction process. The ZT can reach to 2.01 at 320 K Kim, Sang Il, et al. Science 348.6230 (2015): 109-114. scattering cross section Phonon Scattering Mechanism and Electrons Transport within TE Materials Mid / long wavelength phonon Short wavelength phonon • NanostructuredTE materials Hot electrons Cold electrons Two (2-D), one (1-D), zero (0-D) dimensional structure Chen, Zhi-Gang, et al. Progress in Natural Science: Materials International 22.6 (2012): 535- 549.
Methods to Enhance TE Conversion Efficiency • NanostructuredTE materials Schematic illustration of density of states as a function of energy for (a) bulk material, (b) 2-D structure, (c) 1-D structure, (d) 0-D structure Guan, Yonghui, and JingyingXie. "Recent developments in low-dimensional thermoelectric materials."
Methods to Enhance Thermoelectric Conversion Efficiency • Nanostructuring of Thermoelectric materials Table.Typicalexamplesof thermal conductivity k & ZT forNanostructuredThermoelectricmaterials Venkatasubramanian, Rama, et al. Nature 413.6856 (2001): 597-602. Caylor, J. C., et al. Applied physics letters 87.2 (2005): 023105. Broido, D. A., and N. Mingo. Physical Review B 74.19 (2006): 195325. Dresselhaus, Mildred S., et al. Advanced Materials 19.8 (2007): 1043-1053. Boukai, Akram I., et al. Nature 451.7175 (2008): 168-171. D. Harman, T. C., et al. Science 297.5590 (2002): 2229-2232. Hsu, Kuei Fang, et al. Science 303.5659 (2004): 818-821. Poudeu, Pierre FP, et al. AngewandteChemie 118.23 (2006): 3919-3923. Androulakis, John, et al. Journal of the American Chemical Society 129.31 (2007): 9780-9788.
Case Study: Thermoelectric ALD Nanolaminates ofplycrystalline Bi2Te3/ Sb2Te3
Structure of Sb2Te3 / Bi2Te2 • Sb2Te3 and Bi2Te2 are layered chalcogenides with a weak van der Waals-like bonding along their c-axis. • Five layers stacked along c in the sequence Te-Bi-Te-Bi-Te • Both metal tellurides are Te initiated and Te terminated • Te surface lack dangling bonds • The structure cleaves across the c-axis Teweldebrhan, 2010
Influence of Deposition Temperature on The Resulting Morphology & Quality of ALD Sb2Te3 Films 70 C 60 C 65 C 80 C 120 C 180 C These ALD Sb2Te3 films (1000 ALD cycles ) were grown on wet oxide with OHˉ hydroxyl surface groups.
TEM cross-sectional Analysis of ALD laminate of Bi2Te3 and Sb2Te3 (FEI Titan80-300) Energy dispersive X-ray spectroscopy (EDS) analysis identifying the constituents Sb, Bi and Te of the ALD films ALD Bi2Te3 Nanolaminate structure of alternating and Sb2Te3 layers exhibiting localized epitaxial growth as revealed by high resolution TEM X-section analysis. The alternating telluride films grow localized in graphene like fashion in hexagonal layers.
Growth Mechanism of ALD Films of Sb2Te3 • Three basic growth mechanisms for thin film growth: • Volmer – Weber ( Island growth) • Frank Van derMerve (Layer by Layer growth) • Stranski-Krastanov (Layer-by-Layer growth followed by island growth ) • Our experimental data identify Volmer-Weber Island Growth as the growth mechanism for ALD Films of Sb2Te3.
Case Study: Nanoporous Templates for Nanostructuring of thermoelectric ALD Nanolaminates of PbTe/ PbSeEngineering Thermal Transport in Nanostructured Thermoelectric Nanolaminates
ALD Process for Synthesis of PbTe & PbSe Pb(C11H19O2)2 (g) + (Me3Si)2Te (g) ==> PbTe (s) + 2Me3SiC11H19O2(g) Pb(C11H19O2)2 (g) + (Et3Si)2Se (g) ==> PbSe (s) + 2Et3SiC11H19O2(g) • PbTe, PbSe films were grown by ALD on siliconsubstrates using Pb(C11H19O2)2, lead(II)bis(2,2,6,6-tetramethyl3,5-heptanedionato)as the lead precursor, and (Me3Si)2Te,(trimethylsilyl)telluride as the tellurium precursor, and (Et3Si)2Se(triethyl silyl)selane as the selenium precursors. • The lead precursor was heated to 140°C, the telluride precursor to 40°C and the selenium precursor remained at room temperature. • Nitrogen N2 gas was used as a carrier for the precursors. The ALD base chamber pressure was 40 mTorr. • . lead(II)bis(2,2,6,6-tetramethyl-3,5-heptanedionato) (trimethylsilyl)telluride (triethylsilyl)selane
Results and Discussions • TEM Cross-section Micrograph of PbTe Films (a) and (b) Transmission Electron Microscopy (TEM) cross-sectional analysis of ALD deposited PbTe films; (c) low magnification overview of ALD deposited films, (d) and (e) high resolution microstructure of individual PbTe crystallites; and (f) TEM selective area diffraction pattern. • The TEM data is in agreement with XRD, which confirms the presence of poly crystalline PbTe. • The measured lattice constant of 6.440 nm closely matches with the reference value of crystalline PbTe . Zhang, K., H. Baumgartet al. ECS Journal of Solid State Science and Technology 3.6 (2014): P207-P212.
TEM Crosssection Micrograph of PbTe Films Transmission Electron Microscopy (TEM) cross-sectional analysis of ALD deposited PbTe films (a) high resolution microstructure of individual PbTe crystallites, and (b) a fast Fourier transform pattern. • The TEM data is in agreement with XRD, which confirms the presence of poly crystalline PbTe. • The measured lattice constant of 6.440 nm closely matches with the reference value of crystalline PbTe .
PbTe-PbSe Nanolaminate Structure FE-SEM images of basic PbTe-PbSe film structure consisting of 5000 ALD cycles (PbTe) plus 4000 cycles (PbSe) on top of it which may be optimized further into nanolaminate structures (a) planar view and (b) cross-sectional view. • Initially, heterogeneous nucleation sites form and with more ALD cycles the grains grow horizontally and vertically into larger islands. • The initial rock salt structure disappears as islands conglomerate with increased ALD cycles to provide full surface coverage. K. Zhang, H Baumgart et al. ECS Journal of Solid State Science and Technology 3.6 (2014): P207-P212.
Results and Discussions • X-ray Diffraction (XRD) Analysis ofPbTe Film, PbSe Film and Double Layer PbTe/PbSe Film XRD for PbTe (170 ˚C, 2000 cycles) XRD for PbSe (170 ˚C, 4000 cycles) Zhang, K., et al. ECS Journal of Solid State Science and Technology 3.6 (2014): P207-P212. XRD for 5000 cycles PbTe and 4000 cycles PbSe (170 ˚C)
High Angle Annular Dark Field STEM and EDX Spectra and Mapping Results • HAADF-STEM image and the corresponding EDS elemental maps of Pb, Se and Te from the PbTe/PbSe clearly delineates two distinct layers of a basic nanolaminate composite with ALD PbSe on top of ALD PbTe. The orange window marks the area mapped and the yellow window represents the drift correction are used.
Proposed solution ALD Nanolaminates in Porous Templates • Fabricate thermoelectric materials (PbSe, PbTe and PbSe/PbTe superlattices) using conformal coating of high aspect ratio structures to minimize cost and to allow the formation of relatively thick layers of > 200mm by depositing just few 100nm superlatticestructures in periodic Porous Templates. • Si wafer Photolithography RIE/KOH etching Post-treatment Conformal coating of ALD PbTe & PbSe depositions are evaluated
Motivation • Nano-patterning of thermoelectrical materials for Phonon-scattering Engineering Patterning into stripes for subsequent ALD deposition of PbSe layers with different thickness Patterning into porous membranes for subsequent ALD deposition of PbTe/PbSe nanolaminates with different periods
Results and Discussions • Surface Characterization • FE-SEMMicrographsDisplayingSurface Morphology of ALD Synthesized PbSe onStripe patterned SiSubstrates (c) (d) (a) (b) FE-SEM images PbSe film on (a) 1μm, (b) 2 μm, (c) 4 μm patterned Si substrate, (d) cross-sectional images of PbSe film grown on 2 μm wide stripe patterned Si substrate
Results and Discussions • Surface Characterization • FE-SEMMicrographsDisplayingSurface Morphology of ALD Synthesized PbSe/PbTe Nanolaminates inside Porous SiTemplates PbTe / PbSe (10 / 10 nm) nanolaminates was deposited on porous Si substrate by ALD, grown at 150 ˚C. The film thickness is around 170 nm. The misaligned square pores with size of 700 nm (top two figures). The misaligned round square pores with pore size of 3 μm and the width of pore wall of 600 nm (bottom two figures).
Electrical Seebeck Measurements of Nanostructured ALD Nanolaminate Films of PbTe/ PbSe on Nanoporous Si Substrates benchmarked against ALD thermoelectric Films on Planar Si SubstratesTuning Thermal Transport in Nanostructured Thermoelectric Films
Benchmarking: Seebeck Results on Planar Si Substrates Seebeck Measurement of Double Layered ALD PbTe / PbSe Film • Double layered PbTe/PbSe ( 10150 / 10400 cycles ) samples were measured by MMR Seebeck Measurement System. • The Seebeck coefficient in horizontal direction was measured from 300K to 480 K in 20 K interval steps. • The negative Seebeck readings across temperature indicate that the sample is n-type material. • The Seebeck coefficient increases as temperature is increasing, and reaches a maximum value at 460 K, and then decreases as the temperature is further increasing. Seebeck measurement of double layered PbTe/PbSe sample Vineis, C. J., et al. Physical Review B 77.23 (2008): 235202.
Benchmarking: Seebeck Results on Planar Si Substrates Seebeck Measurement of Triple layer ALD Synthesized PbTe/PbSe/PbTe Samples • Triple layered PbTe/PbSe/PbTe samples were measured by MMR Seebeck Measurement System. • The Seebeck coefficient in horizontal direction was measured from 300K to 390 K in 10K steps. • The Seebeck readings as a function of temperature indicate that the material is a p-type. Triple layered ALD PbTe / PbSe / PbTe sample Vineis, C. J., et al. Physical Review B 77.23 (2008): 235202.
New Approach: Seebeck Results on Stripe Patterned Si • Seebeck Coefficient Measurement • Seebeck Measurements of ALD PbSe Synthesized on Stripe patterned Silicon (a) (b) (a) Seebeck coefficient of PbSe films with thickness of 50 nm grown on stripe patterned Si substrate with width of 1 µm and 2 µm and planar SiO2/Si wafer over temperature range of 300 K ~ 500 K in in-plane direction by MMR Seebeck Measurement System. The negative value of Seebeck coefficient indicates the sample is n-type, and charged carriers are electrons. (b) Seebeck coefficient of PbSe film with thickness of 50 nm and 25 nm grown on 2 µm wide stripe patterned Si substrate over temperature range of 300 K ~ 500 K.
New Approach: Seebeck Results on Nanoporous Si Templates • Seebeck Coefficient Measurement • Seebeck Measurements of ALD PbTe / PbSe Nanolaminates Synthesized on Silicon and inside of Porous Si Templates -143.016 ± 5.500 µV/K at 300K -370.556 ± 37.750 µV/K at 300K -574.239 ± 20.79 µV/K at 300K ECS Journal of Solid State Science and Technology, 5(9) 503-508, (2016) Seebeck coefficient of PbTe/PbSe (10 nm/ 10 nm) nanolaminates deposited on (a) Planar Si wafer and (b) microporous Si templates with square pore size of 700 nm and the width of pore wall of 700 nm (c) microporous Si templates with pore size of 3 um and the width of pore wall of 600 nm over the temperature range of 300 K～500 K in in-plane direction by MMR Seebeck Measurement System. The negative value of Seebeck coefficient indicates the sample is n-type, and charged carriers are electrons.
Results and Discussions • Thermal Conductivity Measurement Comparison between Thermoelectric Nanolaminates on Planar Si Substrates and Porous Si Templates • Time Domain Thermo-reflectance (TDTR) 42.8% reduction Thermal conductivity of PbTe/PbSeNanolaminateswith different periods grown on Si wafer and porous silicon template *Collaboration with Dr. V. Kochergin at Micro Xact Inc. at Blacksburg, Virginia. *Collaboration with Prof. P. Hopkins at UVA Charlottesville, Virginia. Table. Thermal conductivity of NL with different periods grown on Si wafer and porous silicon template.
Conclusions • ALD PbSe film was deposited on stripe patterned Si substrate with width of 1 um, 2 um and 4 um. Al2O3 layer with thickness of 20 nm was coated as protections layer. ALD PbTe/PbSe based nanolaminates (NL) TE materials were successfully synthesized on silicon wafer and porous silicon templates. • The width of stripe pattern has a measurable influence on the Seebeck coefficient of PbSe film in horizontal in-plane direction at high temperature. The reduction of film thickness also reveals an improvement of the Seebeck coefficient of PbSe film. • ALD PbTe/PbSe Nanolaminates synthesized inside periodic porous silicon templates exhibit significant higher Seebeck coefficients of 574.239 µV/K in horizontal in-plane direction compared to planar Si substrates. • The thermal conductivity results of ALD PbTe/PbSe NL structure indicate the porous structure contributes to a reduction of the thermal conductivity of the ALD Nanolaminate structure. • The ALD Nanolaminate with lower thickness per layer exhibits lower thermal conductivity. The PbTe/PbSe NL with 20 cycles per layer grown on porous silicon template exhibits lowest thermal conductivity about 0.22 W/(m∙K), resulting from thinner Si pore walls and enhanced phonon scattering by larger density of interfaces from multiple islands and NL layers. • Phonon-boundary engineering is a novel approach to reduce lattice thermal conductivity by nano-patterning ALD thermoelectric films approaching the dimensions of the phonon mean free path, and thus improve the figure of merit of TE materials. • A new method for obtaining high ZT thermoelectric Material by nanostructured ALD is suggested. The path towards obtaining high Power Factor is outlined. • A Novel Approach for growing low thermal conductivity TE material by ALD is demonstrated.